N A N O E X P R E S S
Valence band offset of InN/BaTiO
measured by X-ray photoelectron spectroscopy
, Yonghai Chen1*
, Yan Guo1
, Xianglin Liu1
, Shaoyan Yang1
, Weifeng Zhang2
and Zhanguo Wang1
X-ray photoelectron spectroscopy has been used to measure the valence band offset of the InN/BaTiO3
heterojunction. It is found that a type-I band alignment forms at the interface. The valence band offset (VBO) and conduction band offset (CBO) are determined to be 2.25 ± 0.09 and 0.15 ± 0.09 eV, respectively. The experimental VBO data is well consistent with the value that comes from transitivity rule. The accurate determination of VBO and CBO is important for use of semiconductor/ferrroelectric heterojunction multifunctional devices.
The semiconductor-ferroelectric heterostructures have attracted much attention due to their large potential for new multifunctional electronic and optoelectronic device applications [1-5]. Hysteresis properties of the ferroelec-tric polarization allow for bistable interface polarization configuration The polarization coupling between the fixed permanent semiconductor dipole and the switch-able ferroelectric dipole can be exploited to modify the electronic and the optical properties of a semiconductor heterostructure. Recently, GaN-based high electron mobility transistor devices have been integrated on fer-roelectric LiNbO3, providing the compact
optoelectro-nic/electronic chips with increased cost savings and added functionality . The semiconductor-ZnO/ferro-electric-BaTiO3 (BTO) heterostructure
metal-insulator-semiconductor field-effect transistors have been demon-strated, in which the polarization of the BTO can be used to control the free carrier concentration in the ZnO channel . In order to fully exploit the advantages of semiconductor-ferroelectric heterostructures, other combinations such as InN/BTO should be explored. As a remarkable ferroelectric material with a high relative permittivity, BTO can be used as a gate dielectric for InN-based field-effect transistor. More importantly, InN/BTO heterojunction is promising for fabricating optical and electrical devices since oxidation treatment
is found to reduce the surface electron accumulation of InN films .
For heterostructure devices, it is important to accu-rately determine the valence and the conduction band offsets, which dictate the degree of charge carrier separation and localization. However, up to date, there is lack of experiment data available on the interface band alignment parameters for InN/BTO heterojunc-tion. In this letter, we determine the VBO as well as conduction band offset (CBO) values of the InN/BTO heterojunction using X-ray photoelectron spectroscopy (XPS).
Three samples (bulk BTO, thick InN/BTO, and thin InN/BTO) were studied in this work, namely, a bulk commercial (001) BTO substrate, a thick 200-nm InN layer and a thin 5-nm InN layer grown on the commer-cial (001) BTO substrates, respectively. To get a clean interface, the BTO substrate was cleaned with organic solvents and rinsed with de-ionized water sequentially before loading into the reactor. The thick and thin het-erostructures of InN/BTO were deposited by metal-organic chemical vapor deposition (MOCVD) at 520°C. More growth condition details of the InN layer can be found in our previous report . XPSs were performed on a PHI Quantera SXM instrument with Al Ka (hν = 1486.6 eV) as the X-ray radiation source, which had been carefully calibrated on work function and Fermi energy level (EF). Because a large amount of electrons
are excited and emitted from the sample, the sample is always positively charged and the electric field caused by
* Correspondence: firstname.lastname@example.org
1Key Laboratory of Semiconductor Material Science, Institute of
Semiconductors, Chinese Academy of Science, P.O. Box 912, Beijing 100083, PR China
Full list of author information is available at the end of the article
the charge can affect the measured kinetic energy of photoelectron. Charge neutralization was performed with an electron flood gun and all XPS spectra were calibrated by the C1s peak at 284.8 eV from contamina-tion to compensate the charge effect. Since only the relative energy position in each sample is needed to determine the VBO, the absolute energy calibration for a sample has no effect on the ultimate result. The sur-faces of samples were examined initially by low-resolu-tion survey scans to determine which elements were present. Very high-resolution spectra were acquired to determine the binding energy of core level and the valence band maximum energy in the survey spectra.
Results and discussion
In X-ray θ-2θ diffraction measurements, as shown in Figure 1, the thick InN/BTO sample presented the only peak of InN (0002) reflection and no other InN-related peaks were observed, implying a complete c-axis-oriented growth of the InN layer. The VBO (ΔEV) can
be calculated from the formula
EV=ECL+ (EInNIn3d−E InN
whereECL= (EInN/BTOTi2p −E InN/BTO
In3d )is the energy dif-ference between In3d and Ti2p core levels (CLs) mea-sured in the thin heterojunction InN/BTO, while
Ti2p−EBTOVBM)and(EInNIn3d−EInNVBM)are the valence band maximum (VBM) energies with reference to the CL positions of bulk BTO and thick InN film, respectively. Because all the samples were exposed to air, there must be some impurities (e.g., oxygen and carbon) existing in the sample surface, which may prevent the precise determination of the positions of the VBMs. To reduce
the undesirable effects of surface contamination, all the samples were cleaned by Ar+ bombardment at a low sputtering rate to avoid damage to the samples. After the bombardment, peaks related to impurities were greatly reduced, and no new peaks appeared.
Figure 2 shows the XPS Ti2p and In3d CL narrow scans and the valence band spectra from the bulk BTO, thick InN, and thin InN/BTO samples, respectively. All the CL spectra were fitted to Voigt (mixed Lorentz-Gaussian) line shape with a Shirley background. The uncertainty of the CL position is less than 0.03 eV, eval-uated by numerous fittings with different parameters. The VBM positions were determined by linear extrapo-lation of the leading edge of the VB spectra recorded on the bulk BTO and thick InN film to the base lines to account for the instrument resolution-induced tail . Evidently, the VBM value is sensitive to the choice of points on the leading edge used to obtain the regression line . Several different sets of points were selected over the linear region of the leading edge to perform regressions, and the uncertainty of VBO is found to be less than 0.06 eV in the present work.
For the In3d spectra of both the InN and the thin InN/BTO samples, additional low intensity higher-binding-energy components were required. These extra components are attributed to In-O bonding due to oxide contamination when InN is present at the sur-face , as shown in Figure 2a. In the thin InN/BTO sample shown in Figure 2c, they are attributed to In-O bonding at the InN/BTO interfaces, and/or inelastic losses to free carriers in the InN layer . The CL peak attributed to In-N bonding locates at 443.67 ± 0.03 and 443.98 ± 0.03 eV for thick InN and thin InN/ BTO, respectively, as shown in Figure 2a, c. From Fig-ure 2b, it can be clearly seen that the Ti2p peak in the bulk BTO is not symmetric and consists of two com-ponents by careful Voigt fitting. The prominent one located at 457.12 ± 0.03 eV is attributed to the Ti emitters within the BTO substrate, which have six bonds to oxygen atoms. The other one shifting by ~2 eV to a lower binding energy is attributed to TiOx
suboxides on account of the TiO-terminated BTO initial surface . However, the Ti2p spectrum in the thin InN/BTO heterojunction is quite symmetric, indi-cating a uniform bonding state and the only peaks cor-respond to Ti-O bonds. It is interesting that the Ti2p peaks transform from asymmetry in bulk BTO to sym-metry in the thin InN/BTO sample, as recently observed in the thin ZnO/BTO heterostructure . The VBM value of bulk BTO is determined to be 1.49 ± 0.06 eV using the linear method. The Fermi energy level of an insulator is expected to be located in the middle of the forbidden energy gap, so the VBM will be one-half of the band gap of insulators . For
10 20 30 40 50 60 70 80
Intensity (arb. units.)
BTO, the VBM should be 1.55 eV calculated from the band gap of 3.1 eV , which is in good agreement with the measured value (1.49 ± 0.06 eV) in the pre-sent work. Using the same fitting methods mentioned above, the VBM value for the thick InN lms can be determined to be 0.24 eV, as shown in Figure 1e. Sub-stituting the above values in Equation 1, the resulting VBO value is calculated to be 2.25 ± 0.09 eV.
The reliability of the measured result is analyzed by considering several possible factors that could impact the experiment results. The energy band bends down-ward at the surface of InN film and there is an electron accumulation layer , so the energy separation between VBM and Fermi level can be changed at the InN surface, which could impact the measured VBO values of the heterojunctions. However, both the CL emissions of In3d and Ti2p at the InN/BTO heterojunc-tion are collected from the same surface (InN surface),
thus, the surface band bending effects can be canceled out for the measurement ofΔECL, as was the
measure-ment of the band offset of the InN/AlN heterojunction by others [19,20].
Another factor which may affect the precision of the VBO value is the strain-induced piezoelectric field in the overlayer of the heterojunction . There is a large
lattice mismatch of about 7.1%(
between the hexagonal apothem of InN and the
BTO¯ direction. It is comparable with that of the
InN/ZnO heterojunction (7.7%), and the InN thin film of 5 nm is approximately treated as completely relaxed . So the strain-induced piezoelectric field effect can be neglected in our experiment. Since the factors that can affect the ultimate result can be excluded from the measured result, the experimental obtained VBO value is somewhat reliable.
-2 0 2 4 6 8
1.49 eV (f) BTO: VBM
455 460 465
457.12 eV (b) BTO: Ti 2p
Binding energy (eV)
455 460 465
458.43 eV (d) InN/BTO: Ti 2p
-4 -2 0 2 4 6 8
0.24 eV (e) InN: VBM
440 445 450 455
443.98 eV (c) InN/BTO: In 3d
440 445 450 455
443.67 eV (a) InN: In 3d
To further confirm the reliability of the experimental values, it would be useful to compare our VBO value with other results deduced by transitive property. For heterojunctions formed between all pairs of three mate-rials (A, B, and C),ΔEV(A-C) can be deduced from the
difference betweenΔEV(A-B) and ΔEV(C-B) neglecting
the interface effects . The reported VBO values for ZnO/BTO and InN/ZnO heterojunctions areΔEV
(ZnO-BTO) = 0.48 eV , and ΔEV(InN-ZnO) = 1.76 eV
, respectively. Then theΔEV(InN-BTO) is deduced
to be 2.24 eV, which is well consistent with our mea-sured value 2.25 ± 0.09 eV. In addition, the resulting ΔEV is a large value for device applications which
require strong carrier con nement, such as light emitters or heterostructure field effect transistors.
Finally, the CBO (ΔEC) can be estimated by the
for-mula EC=EBTOg −EInNg −EV. By substituting the band gap values at room temperature (EInNg = 0.7 eV  and EBTOg = 3.1 eV ), ΔEC is calculated to be
0.15 ± 0.09 eV. Accordingly, a type-I band alignment forms at the heterojunction interface, as shown in Figure 3.
In summary, XPS was used to measure the VBO of the InN/BTO heterojunction. A type-I band alignment with the VBO of 2.25 ± 0.09 eV and CBO of 0.15 ± 0.09 eV is obtained. The accurately determined result is impor-tant for the design and application of InN/BTO hetero-structure-based devices.
CBO: conduction band offset; CLs: core levels; MOCVD: metal-organic chemical vapor deposition; VBM: valence band maximum; VBO: valence band offset; XPS: X-ray photoelectron spectroscopy.
This work was supported by the 973 program (2006CB604908, 2006CB921607), and the National Natural Science Foundation of China (60625402, 60990313).
1Key Laboratory of Semiconductor Material Science, Institute of
Semiconductors, Chinese Academy of Science, P.O. Box 912, Beijing 100083, PR China2Key Laboratory of Photovoltaic Materials of Henan Province and
School of Physics Electronics, Henan University, Kaifeng 475004, PR China
CJ carried out the experimental analysis and drafted the manuscript. YC carried out the experimental design. YG participated in the experimental analysis. XL carried out the growth and optimization of indium nitride films. SY participated in the experimental measurement. WZ participated in its design and coordination. ZW participated in the experimental design. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Received: 10 January 2011 Accepted: 8 April 2011 Published: 8 April 2011
1. Voora VM, Hofmann T, Schubert M, Brandt M, Lorenz M, Grundmann M, Ashkenov N, Schubert M:Resistive hysteresis and interface charge coupling in BaTiO3-ZnO heterostructures.Appl Phys Lett2009,94: 142904. 2. Voora VM, Hofmann T, Brandt M, Lorenz M, Grundmann M, Ashkenov N,
Schmidt H, Ianno N, Schbert M:Interface polarization coupling in piezoelectric-semiconductor ferroelectric heterostructures.Phys Rev B
3. Mbenkum BN, Ashkenov N, Schubert M, Lorentz M, Hochmuth H, Michel D, Grundmann M, Wagner G:Temperature-dependent dielectric and electro-optic properties of a ZnO-BaTiO3-ZnO heterostructure grown by pulsed-laser deposition.Appl Phys Lett2005,86: 091904.
4. Losego MD, Kourkoutis LF, Mita S, Craft HS, Muller DA, Collazo R, Sitar Z, Maria JP:Epitaxial Ba0.5Sr0.5TiO3-GaN heterostructures with abrupt interfaces.J Cryst Growth2009,311: 1106.
5. Lorentz M, Brandi M, Schubert J, Hochmuth H, v Wenckstern H, Schubert M, Grundmann M:Polarization coupling in epitaxial ZnO/ BaTiO3thin film heterostructures on SrTiO3(100) substrates.Proc SPIE
6. Namkoong G, Lee KK, Madison SM, Henderson W, Doolittle WA, Ralph SE:
III-nitride integration on ferroelectric materials of lithium niobate by molecular beam epitaxy.Appl Phys Lett2005,87: 171107.
7. Brandt M, Frenzel H, Hochmuth H, Lorentz M, Grundmann M, Schubert J:
Ferroelectric thin film field-effect transistors based on ZnO/BaTiO3 heterostructures.J Vac Sci Technol B2009,27: 1789.
8. Cimalla V, Lebedev V, Wang CY, Ali M, Cke GE, Polyakov VM, Schwierz F, Ambacher O, Lu H, Scha WJ:Reduced surface electron accumulation at InN films by ozone induced oxidation.Appl Phys Lett2007,90: 152106. 9. Jia CH, Chen YH, Zhou XL, Liu GH, Guo Y, Liu XL, Yang SY, Wang ZG:InN
layers grown by MOCVD on SrTiO3substrates.J Cryst Growth2010,312:
10. Zhang RQ, Zhang PF, Kang TT, Fan HB, Liu XL, Yang SY, Wei HY, Zhu QS, Wang ZG:Determination of the valence band offset of wurtzite InN/ZnO heterojunction by x-ray photoelectron spectroscopy.Appl Phys Lett2007,
11. Chambers SA, Droubay T, Kaspar TC, Gutowski M:Experimental determination of valence band maxima for SrTiO3, TiO2, and SrO and the associated valence band offsets with Si(001).J Vac Sci Technol B2004,
12. Piper LFJ, Veal TD, Walker M, Mahboob I, Mcconville CF, Lu H, Scha WJ:
Clean wurtzite InN surfaces prepared with atomic hydrogen.J Vac Sci
Technol A2005,23: 617.
13. King PDC, Veal TD, Lu H, Hatfield SA, Schaff WJ, Mcconville CF:The influence of conduction band plasmons on core-level photoemission spectra of InN.Surf Sci2008,602: 871.
EvBTO EgBTO=3.1 eV EgInN=0.7 eV
(EIn3d-Ev)InN =443.43 eV
(ETi2p-Ev)BTO =455.63 eV
14. Kazzi ME, Merckling C, Delhaye G, Arzel L, Grenet G, Bergignat E, Hollinger G:Photoemission (XPS and XPD) study of epitaxial LaAlO3film grown on SrTiO3(0 0 1).Mater Sci Semicond Process2006,9: 954. 15. Jia CH, Chen YH, Zhou XL, Yang AL, Zheng GL, Liu XL, Yang SY, Wang ZG:
Valence band offset of ZnO/BaTiO3heterojunction measured by X-ray photoelectron spectroscopy.Appl Phys A2010,99: 511.
16. You JB, Zhang XW, Song HP, Ying J, Guo Y, Yang AL, Yin ZG, Chen NF, Zhu QS:Energy band alignment of SiO2/ZnO interface determined by x-ray photoelectron spectroscopy.J Appl Phys2009,106: 043709. 17. Boggess TF, White JO, Valley GC:Two-photon absorption and anisotropic
transient energy transfer in BaTiO3with 1-psec excitation.J Opt Soc Am B1990,7: 2255.
18. Mahboob I, Veal TD, Mcconville CF, Lu H, Scha WJ:Intrinsic Electron Accumulation at Clean InN Surfaces.Phys Rev Lett2004,92: 036804. 19. Wu CL, Shen CH, Gwo S:Valence band offset of wurtzite InN/AlN
heterojunction determined by photoelectron spectroscopy.Appl Phys Lett
20. King PDC, Veal TD, Jefferson PH, Mcconville CF, Wang T, Parbrook PJ, Lu H, Scha WJ:Valence band offset of InN/AlN heterojunctions measured by x-ray photoelectron spectroscopy.Appl Phys Lett2007,90: 132105. 21. Martin G, Botchkarev A, Rockett A, Morkoc H:Valence-band discontinuities
of wurtzite GaN, AlN, and InN heterojunctions measured by x-ray photoemission spectroscopy.Appl Phys Lett1996,68: 2541. 22. Foulon Y, Priester C:Band-offset transitivity in strained (001)
heterointerfaces.Phys Rev B1992,45: 6259.
23. Yang AL, Song HP, Wei HY, Liu XL, Wang J, Lv XQ, Jin P, Yang SY, Zhu QS, Wang ZG:Measurement of polar C-plane and nonpolar A-plane InN/ZnO heterojunctions band offsets by x-ray photoelectron spectroscopy.Appl
Phys Lett2009,94: 163301.
Cite this article as:Jiaet al.:Valence band offset of InN/BaTiO3
heterojunction measured by X-ray photoelectron spectroscopy.
Nanoscale Research Letters20116:316.
Submit your manuscript to a
journal and benefi t from:
7Convenient online submission 7Rigorous peer review
7Immediate publication on acceptance 7Open access: articles freely available online 7High visibility within the fi eld
7Retaining the copyright to your article